Photochemically Cross-Linked Quantum Well Ligands for 2D/3D 2019. 8. 29.¢ Photochemically...
Embed Size (px)
Transcript of Photochemically Cross-Linked Quantum Well Ligands for 2D/3D 2019. 8. 29.¢ Photochemically...
Photochemically Cross-Linked Quantum Well Ligands for 2D/3D Perovskite Photovoltaics with Improved Photovoltage and Stability Andrew H. Proppe,†,‡ Mingyang Wei,‡ Bin Chen,‡ Rafael Quintero-Bermudez,‡ Shana O. Kelley,†,§
and Edward H. Sargent*,‡
†Department of Chemistry and ‡The Edward S. Rogers Department of Electrical and Computer Engineering, University of Toronto, Toronto, Ontario, Canada M5S 3G4 §Department of Pharmaceutical Sciences, Leslie Dan Faculty of Pharmacy, University of Toronto, Toronto, Ontario, Canada M5S 3M2
*S Supporting Information
ABSTRACT: The deployment of perovskite solar cells will rely on further progress in the operating and ambient stability of active layers and interfaces within these materials. Low- dimensional perovskites, also known as perovskite quantum wells (PQWs), utilize organic ligands to protect the perovskite lattice from degradation and offer to improve device stability; combining 2D and 3D perovskites in heterostructures has been shown to take advantage of the high efficiency of the majority 3D active layers and combine it with the improved stability of a thin 2D top layer. Prior PQWs have relied on relatively weak interwell van der Waals bonding between hydrophobic organic moieties of the ligands. Here we instead use the ligand 4-vinylbenzylammonium to form well-ordered PQWs atop a 3D perovskite layer. The ligand’s vinyl group is activated using UV light which photochemically forms new covalent bonds among PQWs. UV-cross-linked 2D/3D devices show improved operational stability as well as improved long- term dark stability in air: they retain 90% of their initial efficiency after 2300 h of dark aging compared to a retention of 20% of performance in the case of 3D films. The UV-cross-linked PQWs and 2D/3D interfaces reduce device hysteresis and improve the open-circuit voltages to values up to 1.20 V, resulting in more efficient devices (PCE of up to 20.4%). This work highlights the exploitation of the chemical reactivity of PQW ligands to tailor the molecular properties of PQW interfaces for improved stability and performance in 2D/3D perovskite photovoltaics.
■ INTRODUCTION Metal halide perovskites have recently reached certified power conversion efficiencies (PCEs) above 24% for single junction devices1,2 and an impressive 28% for monolithic perovskite− silicon tandems.3 A remaining opportunity is to understand and improve perovskite solar cell stability further. The dark (i.e., shelf life) and operational stability of perovskite solar cells have seen tremendous improvements in recent years.4−7
However, most reported metrics still fall short of the industry standard accelerated aging conditions used to assess the long- term operating stability of a solar cell.8
Low-dimensional perovskites, or perovskite quantum wells (PQWs), are quasi-two-dimensional analogues of the bulk 3D perovskite structure where organic ligand molecules terminate the lattice along one axis into a finite number of monolayers, n.7,9,10 The hydrophobic organic ligands form bilayer interfaces that repel water and increase the formation energy of the PQWs relative to the 3D structures,11,12 increasing thermal stability,13 helping prevent moisture-induced decomposi- tion,14,15 and reducing migration of labile ions within the material.16 This has been shown to enhance the ambient and
operating lifetimes for photovoltaic devices based on these materials.7,11,12,17 More recently, stacked 2D/3D heterostruc- tures consisting of a thin layer of PQWs atop a majority 3D perovskite active layer have seen success in combining the stability of PQWs with the exceptional optoelectronic properties of bulk perovskites, enabling solar cells with PCEs near or above 20% that possess superior operating and ambient stability compared to 3D-only devices.2,13,18
Many types of alkyl- and arylammonium ligands have been explored in PQWs.7,14,19−22 The molecular interfaces between wells are composed of interdigitating ligands that are stabilized by van der Waals interactions, which increases their desorption energy compared to the smaller cations like methylammonium and results in an overall stabilization of the perovskite material.11 Typically, short chain ligands such as phenethyl- ammonium11,23,24 or butylammonium7,9 are desired to minimize the inter-PQW distance so as to not impede interwell charge transfer.25,26 Extending the degree of van
Received: May 12, 2019 Published: August 17, 2019
pubs.acs.org/JACSCite This: J. Am. Chem. Soc. XXXX, XXX, XXX−XXX
© XXXX American Chemical Society A DOI: 10.1021/jacs.9b05083 J. Am. Chem. Soc. XXXX, XXX, XXX−XXX
us t 2
pubs.acs.org/JACS http://pubs.acs.org/action/showCitFormats?doi=10.1021/jacs.9b05083 http://dx.doi.org/10.1021/jacs.9b05083
der Waals stabilization, for example, by increasing ligand length to achieve more interdigitation, thus results in a compromise to device performance by reducing the efficiency of charge transport through these interfaces. Passarelli et al. have demonstrated 2D perovskites with remarkable stability that could even withstand full immersion in water, but these required large ether-linked pyrene ligands with extended π−π interactions to achieve such stabilization, severely limiting interwell charge transfer and their utility in high efficiency photovoltaics.19
In a recent report, Li et al. used a molecular additive trimethylolpropane triacrylateto anchor to grain boundaries and undergo thermally induced chemical cross-linking.27 The resulting films had improved operational stability under ambient conditions as well as upon exposure to high temperature and humidity. Here we took the view that a cross-linking approach could
be applied to stabilize the interfaces of PQWs. Functionalizing small molecule ligandsin order not to compromise perform- ancesuch that they could be activated after the formation of the PQW interfaces would go beyond the van der Waals stabilization of perovskite ligands by forming stronger covalent bonds among neighboring PQWs. Early work by Tieke et al. showed that trans-butadiene ammonium ligands, used to form layered cadmium chloride perovskites, could be photo- polymerized following UV irradiation while retaining the 2D perovskite structure.28,29 More recent work by Ortiz-Cervantes et al. demonstrated thermally cross-linked dialkynyl ligands in 2D lead halide perovskites, where the polymerized interfaces improved the conductivity by 3 orders of magnitude and could be used to control the bandgap and doping properties of the hybrid material.30
To build on these seminal works and use cross-linkable ligands in high efficiency 2D/3D solar cells, we selected the ligand 4-vinylbenzylammonium (VBA). VBA is ideally suited for this application because it has a highly similar structure to phenethylammoniumwhich has been used extensively in PQW devicesbut bears an additional terminal vinyl group in the para position of the aromatic phenyl ring. This extended conjugation facilitates absorption of ultraviolet light (∼250 nm) by the vinylbenzyl moiety,31 allowing for direct photo- excitation to trigger photochemical cross-linking.32 We used VBA to form well-ordered n = 1 and n = 2 PQWs atop a 3D active layer in a 2D/3D heterostructure, whereafter exposure of the top layer to UV photoexcitation activates the vinyl groups of VBA to form new covalent bonds among the 2D layers. The cross-linked 2D/3D heterostructure (hereafter termed 2D-x/ 3D) exhibits improved open-circuit voltages and negligible current−voltage hysteresis compared to the 3D-only devices, resulting in PCEs exceeding 20%. The 2D-x/3D devices also exhibit much better stability in air compared to the 3D-only and non-cross-linked 2D/3D devices, consistent with new covalent bonds helping further stabilize the PQW interfaces. This work demonstrates how the stability gained from employing Ruddlesden−Popper perovskites in 2D/3D hetero- structures can be further augmented using photochemically reactive ligands in order form new interwell covalent bonds among the well-ordered PQWs.
■ RESULTS AND DISCUSSION An illustration of the formation of cross-linked 2D-x/3D perovskite heterostructures is shown in Figure 1. First, a 3D p e r o v s k i t e fi l m w i t h t h e c o m p o s i t i o n (MAPbBr3)0.15(FAPbI3)0.85 (containing 5% of Cs) is spin-
Figure 1. Formation and optical properties of 2D/3D heterostructures using the ligand VBABr. (a) Schematic illustrating the process by which formation of cross-linked 2D perovskites atop a 3D majority layer is achieved using the ligand 4-vinylbenzylammonium bromide (VBABr). The new bonds formed following photochemical cross-linking are left ambiguous in this illustration and discussed in more detail below. (b) Energy level diagram for the 2D/3D interface. Valence band-edge values are extracted from UPS measurements on 3D-only and 2D-x/3D films (with various UV exposure times). (c) Absorption spectra, (d) photoluminescence emission spectra, and (e) TCSPC data for thin films of the 3D and 2D/3D perovskites. PL and TCSPC measurements are performed on both the front (f) and back (b) sides of the fil